Topological Control in Heterometallic Metal-Organic Frameworks by Anion Templating and Metalloligand Design
Sara R. Halper; Loi Do; Jay R. Stork; Seth M. Cohen; Journal of the American Chemical Society 128 (2006) 15255–15268; doi:10.1021/ja0645483

data_4111126
_publ_section_title
;
 Topological Control in Heterometallic Metal-Organic Frameworks by Anion
 Templating and Metalloligand Design
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              15255
_journal_page_last               15268
_journal_paper_doi               10.1021/ja0645483
_journal_volume                  128
_journal_year                    2006
_chemical_formula_moiety
'C42 H30 Ag Fe N9, C2 H3 N, F6 Sb, 1.5(C6 H6)'
_chemical_formula_sum            'C53 H42 Ag F6 Fe N10 Sb'
_chemical_formula_weight         1218.44
_chemical_name_common            MOF-Fe/AgSbF~6~-1
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 110.009(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   15.874(2)
_cell_length_b                   24.606(3)
_cell_length_c                   16.377(2)
_cell_measurement_reflns_used    9154
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      24.6
_cell_measurement_theta_min      2.26
_cell_volume                     6010.7(13)
_computing_cell_refinement       SMART
_computing_data_collection       'SMART 5.054 (Bruker, 2003)'
_computing_data_reduction        'SAINT 6.45A (Bruker, 2003)'
_computing_molecular_graphics    'SHELXTL 5.1 (Sheldrick, 1994)'
_computing_publication_material  SHELXL97
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean 8.3
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker APEX'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0622
_diffrn_reflns_av_sigmaI/netI    0.0616
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       29
_diffrn_reflns_limit_k_min       -29
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            44457
_diffrn_reflns_theta_full        25.35
_diffrn_reflns_theta_max         25.35
_diffrn_reflns_theta_min         1.37
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    1.065
_exptl_absorpt_correction_T_max  0.96781
_exptl_absorpt_correction_T_min  0.82314
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS 2.10 (Sheldrick, 2004)'
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    1.346
_exptl_crystal_description       plate
_exptl_crystal_F_000             2432
_exptl_crystal_size_max          0.22
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.04
_platon_squeeze_details          ' ?'
_refine_diff_density_max         1.012
_refine_diff_density_min         -0.805
_refine_diff_density_rms         0.134
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.078
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     683
_refine_ls_number_reflns         10996
_refine_ls_number_restraints     17
_refine_ls_restrained_S_all      1.078
_refine_ls_R_factor_all          0.1297
_refine_ls_R_factor_gt           0.1070
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0848P)^2^+59.4350P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2651
_refine_ls_wR_factor_ref         0.2759
_reflns_number_gt                7990
_reflns_number_total             10996
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            ja0645483rom20060627_113302_02.cif
_cod_data_source_block           MOF-Fe/AgSbF~6~-1
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               4111126